# Normalized and Tempered (+NT) 1.0625 Steel

EN 1.0625 +NT steel is EN 1.0625 steel in the normalized and tempered condition. The graph bars on the material properties cards below compare EN 1.0625 +NT steel to: cast carbon steels (top), all iron alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Elastic (Young's, Tensile) Modulus

190 *GPa* 27 *x 10 ^{6} psi*

Elongation at Break

25 *%*

Fatigue Strength

230 *MPa* 34 *x 10 ^{3} psi*

Impact Strength: V-Notched Charpy

30 *J* 22 *ft-lb*

Poisson's Ratio

0.29

Shear Modulus

73 *GPa* 11 *x 10 ^{6} psi*

Tensile Strength: Ultimate (UTS)

560 *MPa* 81 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

320 *MPa* 46 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

250 *J/g*

Maximum Temperature: Mechanical

400 *°C* 750 *°F*

Melting Completion (Liquidus)

1460 *°C* 2660 *°F*

Melting Onset (Solidus)

1420 *°C* 2580 *°F*

Specific Heat Capacity

470 *J/kg-K* 0.11 *BTU/lb-°F*

Thermal Conductivity

47 *W/m-K* 27 *BTU/h-ft-°F*

Thermal Expansion

12 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

7.3 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

8.4 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

2.2 *% relative*

Density

7.8 *g/cm ^{3}* 490

*lb/ft*

^{3}Embodied Carbon

1.5 *kg CO _{2}/kg material*

Embodied Energy

20 *MJ/kg* 8.5 *x 10 ^{3} BTU/lb*

Embodied Water

48 *L/kg* 5.8 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

120 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

270 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

24 *points*

Strength to Weight: Axial

20 *points*

Strength to Weight: Bending

19 *points*

Thermal Diffusivity

13 *mm ^{2}/s*

Thermal Shock Resistance

18 *points*

## Alloy Composition

Fe | 96.6 to 99.02 | |

Mn | 0.8 to 1.4 | |

Si | 0 to 0.6 | |

C | 0.18 to 0.25 | |

Ni | 0 to 0.4 | |

Cr | 0 to 0.3 | |

Cu | 0 to 0.3 | |

Mo | 0 to 0.12 | |

P | 0 to 0.030 | |

V | 0 to 0.030 | |

S | 0 to 0.020 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Further Reading

ISO 4991: Steel castings for pressure purposes

Carbon Steel Handbook, D. Gandy, 2007

Ferrous Materials: Steel and Cast Iron, Hans Berns and Werner Theisen, 2008

Steels: Processing, Structure, and Performance, 2nd ed., George Krauss, 2015